#------------------------------------------------------------------------------
#$Date: 2016-03-26 14:08:46 +0200 (Sat, 26 Mar 2016) $
#$Revision: 180249 $
#$URL: svn://www.crystallography.net/cod/cif/7/11/35/7113566.cif $
#------------------------------------------------------------------------------
#
# This file is available in the Crystallography Open Database (COD),
# http://www.crystallography.net/
#
# All data on this site have been placed in the public domain by the
# contributors.
#
data_7113566
loop_
_publ_author_name
'Rather, Beth'
'Zaworotko, Michael J.'
_publ_section_title
;
 A 3D metal-organic network, [Cu2(glutarate)2(4,4′-bipyridine)],
 that exhibits single-crystal to single-crystal dehydration and
 rehydrationElectronic supplementary information (ESI) available:
 experimental details, IR, TGA and XRPD of all compounds. See
 http://www.rsc.org/suppdata/cc/b3/b301219k/.
;
_journal_issue                   7
_journal_name_full               'Chemical Communications'
_journal_page_first              830
_journal_paper_doi               10.1039/b301219k
_journal_year                    2003
_chemical_formula_moiety         '(C20 H20 Cu2 N2 O8)n,3n(H2 O1)'
_chemical_formula_sum            'C20 H20 Cu2 N2 O11'
_chemical_formula_weight         591.46
_chemical_name_systematic
; 
? 
;
_space_group_IT_number           15
_symmetry_cell_setting           monoclinic
_symmetry_space_group_name_Hall  '-C 2yc'
_symmetry_space_group_name_H-M   'C 1 2/c 1'
_atom_sites_solution_hydrogens   geom
_atom_sites_solution_primary     direct
_atom_sites_solution_secondary   difmap
_audit_creation_method           SHELXL-97
_cell_angle_alpha                90.00
_cell_angle_beta                 101.007(2)
_cell_angle_gamma                90.00
_cell_formula_units_Z            4
_cell_length_a                   21.351(2)
_cell_length_b                   13.1381(13)
_cell_length_c                   8.5699(9)
_cell_measurement_reflns_used    4335
_cell_measurement_temperature    100(2)
_cell_measurement_theta_max      27.11
_cell_measurement_theta_min      2.80
_cell_volume                     2359.7(4)
_computing_cell_refinement       'Bruker SMART'
_computing_data_collection       'Bruker SMART'
_computing_data_reduction        'Bruker SAINT'
_computing_molecular_graphics    'Bruker SHELXTL'
_computing_publication_material  'Bruker SHELXTL'
_computing_structure_refinement  'SHELXL-97 (Sheldrick, 1997)'
_computing_structure_solution    'SHELXS-97 (Sheldrick, 1990)'
_diffrn_ambient_temperature      100(2)
_diffrn_measured_fraction_theta_full 0.993
_diffrn_measured_fraction_theta_max 0.993
_diffrn_measurement_device_type  'CCD area detector'
_diffrn_measurement_method       'phi and omega scans'
_diffrn_radiation_monochromator  graphite
_diffrn_radiation_source         'fine-focus sealed tube'
_diffrn_radiation_type           MoK\a
_diffrn_radiation_wavelength     0.71073
_diffrn_reflns_av_R_equivalents  0.0304
_diffrn_reflns_av_sigmaI/netI    0.0387
_diffrn_reflns_limit_h_max       27
_diffrn_reflns_limit_h_min       -27
_diffrn_reflns_limit_k_max       16
_diffrn_reflns_limit_k_min       -9
_diffrn_reflns_limit_l_max       10
_diffrn_reflns_limit_l_min       -10
_diffrn_reflns_number            6920
_diffrn_reflns_theta_full        27.12
_diffrn_reflns_theta_max         27.12
_diffrn_reflns_theta_min         1.83
_exptl_absorpt_coefficient_mu    1.864
_exptl_absorpt_correction_T_max  1.0000
_exptl_absorpt_correction_T_min  0.8057
_exptl_absorpt_correction_type   SADABS
_exptl_crystal_colour            green
_exptl_crystal_density_diffrn    1.665
_exptl_crystal_density_meas      0
_exptl_crystal_density_method    'not measured'
_exptl_crystal_description       diamondoid
_exptl_crystal_F_000             1200
_exptl_crystal_size_max          0.08
_exptl_crystal_size_mid          0.08
_exptl_crystal_size_min          0.08
_refine_diff_density_max         0.628
_refine_diff_density_min         -0.328
_refine_diff_density_rms         0.111
_refine_ls_extinction_method     none
_refine_ls_goodness_of_fit_ref   1.094
_refine_ls_hydrogen_treatment    mixed
_refine_ls_matrix_type           full
_refine_ls_number_parameters     182
_refine_ls_number_reflns         2582
_refine_ls_number_restraints     0
_refine_ls_restrained_S_all      1.094
_refine_ls_R_factor_all          0.0465
_refine_ls_R_factor_gt           0.0380
_refine_ls_shift/su_max          0.000
_refine_ls_shift/su_mean         0.000
_refine_ls_structure_factor_coef Fsqd
_refine_ls_weighting_details
'calc w=1/[σ²(Fo²)+(0.0637P)²+3.7481P] where P=(Fo²+2Fc²)/3'
_refine_ls_weighting_scheme      calc
_refine_ls_wR_factor_gt          0.1071
_refine_ls_wR_factor_ref         0.1112
_reflns_number_gt                2227
_reflns_number_total             2582
_reflns_threshold_expression     >2sigma(I)
_cod_data_source_file            b301219k.txt
_cod_data_source_block           compound1c
_cod_depositor_comments
;
The following automatic conversions were performed:

'_symmetry_cell_setting' value 'Monoclinic' changed to 'monoclinic'
according to
/usr/data/users/saulius/automatic-downloads/retrospective/RSC/lib/dictionaries/cif_core.dic
dictionary named 'cif_core.dic' version 2.4.2 from 2011-04-26.

Automatic conversion script
Id: cif_fix_values 2281 2013-09-26 08:29:07Z andrius 
;
_cod_original_cell_volume        2359.8(4)
_cod_original_sg_symbol_H-M      C2/c
_cod_database_code               7113566
loop_
_symmetry_equiv_pos_as_xyz
'x, y, z'
'-x, y, -z+1/2'
'x+1/2, y+1/2, z'
'-x+1/2, y+1/2, -z+1/2'
'-x, -y, -z'
'x, -y, z-1/2'
'-x+1/2, -y+1/2, -z'
'x+1/2, -y+1/2, z-1/2'
loop_
_atom_site_label
_atom_site_type_symbol
_atom_site_fract_x
_atom_site_fract_y
_atom_site_fract_z
_atom_site_U_iso_or_equiv
_atom_site_adp_type
_atom_site_occupancy
_atom_site_symmetry_multiplicity
_atom_site_calc_flag
_atom_site_refinement_flags
Cu1 Cu 0.302182(15) 0.29456(3) 0.07568(4) 0.01228(14) Uani 1 1 d .
N1 N 0.37958(11) 0.3723(2) 0.2283(3) 0.0164(5) Uani 1 1 d .
O1 O 0.33266(10) 0.15573(16) 0.1346(3) 0.0184(5) Uani 1 1 d .
O2 O 0.24366(10) 0.08061(16) 0.0091(3) 0.0211(5) Uani 1 1 d .
O3 O 0.24667(10) -0.20829(16) 0.2512(3) 0.0184(5) Uani 1 1 d .
O4 O 0.33698(11) -0.27828(17) 0.3801(3) 0.0217(5) Uani 1 1 d .
C1 C 0.29854(14) 0.0790(2) 0.0941(3) 0.0146(6) Uani 1 1 d .
C2 C 0.32458(15) -0.0224(2) 0.1583(3) 0.0173(6) Uani 1 1 d .
H2A H 0.3058 -0.0392 0.2522 0.021 Uiso 1 1 calc R
H2B H 0.3712 -0.0156 0.1951 0.021 Uiso 1 1 calc R
C3 C 0.31212(15) -0.1107(2) 0.0414(3) 0.0172(6) Uani 1 1 d .
H3A H 0.3346 -0.0981 -0.0476 0.021 Uiso 1 1 calc R
H3B H 0.2658 -0.1147 -0.0030 0.021 Uiso 1 1 calc R
C4 C 0.33457(15) -0.2124(2) 0.1204(4) 0.0171(6) Uani 1 1 d .
H4A H 0.3244 -0.2677 0.0412 0.020 Uiso 1 1 calc R
H4B H 0.3815 -0.2106 0.1561 0.020 Uiso 1 1 calc R
C5 C 0.30359(14) -0.2352(2) 0.2614(3) 0.0149(6) Uani 1 1 d .
C6 C 0.38007(17) 0.4726(3) 0.2419(5) 0.0393(11) Uani 1 1 d .
H6 H 0.3473 0.5104 0.1764 0.047 Uiso 1 1 calc R
C7 C 0.42610(19) 0.5249(3) 0.3469(6) 0.0469(13) Uani 1 1 d .
H7 H 0.4244 0.5971 0.3521 0.056 Uiso 1 1 calc R
C8 C 0.47442(14) 0.4730(2) 0.4440(3) 0.0166(6) Uani 1 1 d .
C9 C 0.47312(17) 0.3688(3) 0.4310(4) 0.0301(8) Uani 1 1 d .
H9 H 0.5050 0.3289 0.4956 0.036 Uiso 1 1 calc R
C10 C 0.42512(18) 0.3222(3) 0.3233(4) 0.0305(8) Uani 1 1 d .
H10 H 0.4250 0.2500 0.3175 0.037 Uiso 1 1 calc R
O1AW O 0.5000 0.902(5) 0.2500 0.220(17) Uani 0.50 2 d SP
O1BW O 0.5000 1.0335(18) 0.2500 0.213(18) Uani 0.50 2 d SP
O2W O 0.5065(13) 0.899(4) 0.085(6) 0.23(3) Uani 0.33 1 d P
O3W O 0.5416(6) 0.8683(13) -0.027(3) 0.143(9) Uani 0.33 1 d P
O4W O 0.4988(15) 0.975(3) 0.156(13) 0.53(12) Uani 0.33 1 d P
loop_
_atom_type_symbol
_atom_type_description
_atom_type_scat_dispersion_real
_atom_type_scat_dispersion_imag
_atom_type_scat_source
C C 0.0033 0.0016 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
H H 0.0000 0.0000 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
N N 0.0061 0.0033 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
O O 0.0106 0.0060 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Cu Cu 0.3201 1.2651 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
loop_
_geom_angle_atom_site_label_1
_geom_angle_atom_site_label_2
_geom_angle_atom_site_label_3
_geom_angle
_geom_angle_site_symmetry_1
_geom_angle_site_symmetry_3
O1 Cu1 O3 89.20(9) . 4
O1 Cu1 O4 87.57(10) . 6
O3 Cu1 O4 168.05(9) 4 6
O1 Cu1 O2 168.26(8) . 7
O3 Cu1 O2 89.78(10) 4 7
O4 Cu1 O2 91.05(10) 6 7
O1 Cu1 N1 96.08(9) . .
O3 Cu1 N1 90.39(9) 4 .
O4 Cu1 N1 101.39(9) 6 .
O2 Cu1 N1 95.62(9) 7 .
O1 Cu1 Cu1 85.49(6) . 7
O3 Cu1 Cu1 80.92(6) 4 7
O4 Cu1 Cu1 87.35(6) 6 7
O2 Cu1 Cu1 82.80(6) 7 7
N1 Cu1 Cu1 171.17(7) . 7
C10 N1 C6 116.8(3) . .
C10 N1 Cu1 121.8(2) . .
C6 N1 Cu1 121.1(2) . .
C1 O1 Cu1 121.87(19) . .
C1 O2 Cu1 124.7(2) . 7
C5 O3 Cu1 126.8(2) . 4_545
C5 O4 Cu1 119.3(2) . 6_556
O1 C1 O2 125.1(3) . .
O1 C1 C2 117.1(2) . .
O2 C1 C2 117.8(3) . .
C1 C2 C3 115.3(2) . .
C2 C3 C4 111.9(2) . .
C5 C4 C3 112.2(2) . .
O3 C5 O4 125.1(3) . .
O3 C5 C4 117.0(3) . .
O4 C5 C4 117.9(3) . .
N1 C6 C7 123.1(3) . .
C8 C7 C6 120.3(3) . .
C9 C8 C7 116.3(3) . .
C9 C8 C8 121.9(3) . 5_666
C7 C8 C8 121.8(4) . 5_666
C8 C9 C10 119.7(3) . .
N1 C10 C9 123.8(3) . .
O4W O1AW O4W 80(10) 2_655 .
O4W O1AW O2W 131(9) 2_655 .
O4W O1AW O2W 52(3) . .
O4W O1AW O2W 52(3) 2_655 2_655
O4W O1AW O2W 131(9) . 2_655
O2W O1AW O2W 177(8) . 2_655
O4W O1AW O1BW 40(5) 2_655 .
O4W O1AW O1BW 40(5) . .
O2W O1AW O1BW 91(4) . .
O2W O1AW O1BW 91(4) 2_655 .
O4W O1BW O4W 92(10) . 2_655
O4W O1BW O1AW 46(5) . .
O4W O1BW O1AW 46(5) 2_655 .
O4W O2W O3W 138(8) . .
O4W O2W O1AW 55(5) . .
O3W O2W O1AW 148(4) . .
O1BW O4W O2W 164(9) . .
O1BW O4W O1AW 94(10) . .
O2W O4W O1AW 73(4) . .
O1BW O4W O4W 44(5) . 2_655
O2W O4W O4W 122(7) . 2_655
O1AW O4W O4W 50(5) . 2_655
loop_
_geom_bond_atom_site_label_1
_geom_bond_atom_site_label_2
_geom_bond_distance
_geom_bond_site_symmetry_2
Cu1 O1 1.970(2) .
Cu1 O3 1.970(2) 4
Cu1 O4 1.970(2) 6
Cu1 O2 1.976(2) 7
Cu1 N1 2.159(2) .
Cu1 Cu1 2.6297(7) 7
N1 C10 1.319(4) .
N1 C6 1.322(4) .
O1 C1 1.254(4) .
O2 C1 1.256(3) .
O2 Cu1 1.976(2) 7
O3 C5 1.253(4) .
O3 Cu1 1.970(2) 4_545
O4 C5 1.260(4) .
O4 Cu1 1.970(2) 6_556
C1 C2 1.505(4) .
C2 C3 1.523(4) .
C3 C4 1.532(4) .
C4 C5 1.514(4) .
C6 C7 1.382(5) .
C7 C8 1.376(5) .
C8 C9 1.373(4) .
C8 C8 1.489(5) 5_666
C9 C10 1.384(4) .
O1AW O4W 1.24(8) 2_655
O1AW O4W 1.24(8) .
O1AW O2W 1.45(5) .
O1AW O2W 1.45(5) 2_655
O1AW O1BW 1.73(6) .
O1BW O4W 1.12(7) .
O1BW O4W 1.12(7) 2_655
O2W O4W 1.19(5) .
O2W O3W 1.38(4) .
O4W O4W 1.6(2) 2_655
loop_
_geom_torsion_atom_site_label_1
_geom_torsion_atom_site_label_2
_geom_torsion_atom_site_label_3
_geom_torsion_atom_site_label_4
_geom_torsion
C1 C2 C3 C4 -174.7(3)
C2 C3 C4 C5 57.1(3)
